Red copper oxide
3D model (JSmol)
CompTox Dashboard (EPA)
|Molar mass||143.09 g/mol|
|Melting point||1,232 °C (2,250 °F; 1,505 K)|
|Boiling point||1,800 °C (3,270 °F; 2,070 K)|
|Solubility in acid||Soluble|
|Band gap||2.137 eV|
a = 4.2696
Std enthalpy of
|Safety data sheet||SIRI.org|
|GHS Signal word||Danger|
|H302, H318, H332, H400, H410|
|NFPA 704 (fire diamond)|
|NIOSH (US health exposure limits):|
|TWA 1 mg/m3 (as Cu)|
|TWA 1 mg/m3 (as Cu)|
IDLH (Immediate danger)
|TWA 100 mg/m3 (as Cu)|
Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).
|what is ?)(|
Copper(I) oxide or cuprous oxide is the inorganic compound with the formula Cu2O. It is one of the principal oxides of copper, the other being or copper(II) oxide or cupric oxide (CuO). This red-coloured solid is a component of some antifouling paints. The compound can appear either yellow or red, depending on the size of the particles. Copper(I) oxide is found as the reddish mineral cuprite.
Copper(I) oxide may be produced by several methods. Most straightforwardly, it arises via the oxidation of copper metal:
- 4 Cu + O2 → 2 Cu2O
Additives such as water and acids affect the rate of this process as well as the further oxidation to copper(II) oxides. It is also produced commercially by reduction of copper(II) solutions with sulfur dioxide. Aqueous cuprous chloride solutions react with base to give the same material. In all cases, the color is highly sensitive to the procedural details.
Formation of copper(I) oxide is the basis of the Fehling's test and Benedict's test for reducing sugars. These sugars reduce an alkaline solution of a copper(II) salt, giving a bright red precipitate of Cu2O.
Little evidence exists for copper(I) hydroxide CuOH, which is expected to rapidly undergo dehydration. A similar situation applies to the hydroxides of gold(I) and silver(I).
The solid is diamagnetic. In terms of their coordination spheres, copper centres are 2-coordinated and the oxides are tetrahedral. The structure thus resembles in some sense the main polymorphs of SiO2, and both structures feature interpenetrated lattices.
Copper(I) oxide dissolves in concentrated ammonia solution to form the colourless complex [Cu(NH3)2]+, which is easily oxidized in air to the blue [Cu(NH3)4(H2O)2]2+. It dissolves in hydrochloric acid to give solutions of CuCl−
2. Dilute sulfuric acid and nitric acid produce copper(II) sulfate and copper(II) nitrate, respectively.
Cu2O degrades to copper(II) oxide in moist air.
Cu2O crystallizes in a cubic structure with a lattice constant al = 4.2696 Å. The copper atoms arrange in a fcc sublattice, the oxygen atoms in a bcc sublattice. One sublattice is shifted by a quarter of the body diagonal. The space group is Pn3m, which includes the point group with full octahedral symmetry.
In the history of semiconductor physics, Cu2O is one of the most studied materials, and many experimental semiconductor applications have been demonstrated first in this material:
- Semiconductor diodes
- Phonoritons ("a coherent superposition of exciton, photon, and phonon")
The lowest excitons in Cu2O are extremely long lived; absorption lineshapes have been demonstrated with neV linewidths, which is the narrowest bulk exciton resonance ever observed. The associated quadrupole polaritons have low group velocity approaching the speed of sound. Thus, light moves almost as slowly as sound in this medium, which results in high polariton densities. Another unusual feature of the ground state excitons is that all primary scattering mechanisms are known quantitatively. Cu2O was the first substance where an entirely parameter-free model of absorption linewidth broadening by temperature could be established, allowing the corresponding absorption coefficient to be deduced. It can be shown using Cu2O that the Kramers–Kronig relations do not apply to polaritons.
Cuprous oxide is commonly used as a pigment, a fungicide, and an antifouling agent for marine paints. Rectifier diodes based on this material have been used industrially as early as 1924, long before silicon became the standard. Copper(I) oxide is also responsible for the pink color in a positive Benedict's test.
- NIOSH Pocket Guide to Chemical Hazards. "#0150". National Institute for Occupational Safety and Health (NIOSH).
- N. N. Greenwood, A. Earnshaw, Chemistry of the Elements, 2nd ed., Butterworth-Heinemann, Oxford, UK, 1997.
- H. Wayne Richardson "Copper Compounds in Ullmann's Encyclopedia of Industrial Chemistry 2002, Wiley-VCH, Weinheim. doi:10.1002/14356007.a07_567
- D. Nicholls, Complexes and First-Row Transition Elements, Macmillan Press, London, 1973.
- L. O. Grondahl, Unidirectional current carrying device, Patent, 1927
- Hanke, L.; Fröhlich, D.; Ivanov, A. L.; Littlewood, P. B.; Stolz, H. (1999-11-22). "LA Phonoritons in Cu2O". Physical Review Letters. 83 (21): 4365–4368. doi:10.1103/PhysRevLett.83.4365.
- L. Brillouin: Wave Propagation and Group Velocity, Academic Press, New York City, 1960 ISBN 9781483276014.
- Brandt, Jan; Fröhlich, Dietmar; Sandfort, Christian; Bayer, Manfred; Stolz, Heinrich; Naka, Nobuko (2007-11-19). "Ultranarrow Optical Absorption and Two-Phonon Excitation Spectroscopy of Cu2O Paraexcitons in a High Magnetic Field". Physical Review Letters. American Physical Society (APS). 99 (21): 217403. doi:10.1103/physrevlett.99.217403. ISSN 0031-9007.
- J. P. Wolfe and A. Mysyrowicz: Excitonic Matter, Scientific American 250 (1984), No. 3, 98.
- Hopfield, J. J. (1958). "Theory of the Contribution of Excitons to the Complex Dielectric Constant of Crystals". Physical Review. 112 (5): 1555–1567. doi:10.1103/PhysRev.112.1555. ISSN 0031-899X.
|Wikimedia Commons has media related to Copper(I) oxide.|